# Ch-5 Sheet Metal Operation.pdf

8 de May de 2022
1 de 20

### Ch-5 Sheet Metal Operation.pdf

• 1. 7/14/2015 1 Sheet Metal Operation Sheet Metal  Product has light weight and versatile shape as compared to forging/casting  Most commonly used – low carbon steel sheet (cost, strength, formability)  Aluminium and titanium for aircraft and aerospace  Sheet metal has become a significant material for, - automotive bodies and frames, - office furniture - frames for home appliances Piercing (Punching) and Blanking  Piercing and blanking are shearing operations.  In blanking, the piece being punched out becomes the workpiece and any major burrs or undesirable featuresshould be left on the remaining strip.  In piercing (Punching), the punch-out is the scrap and the remaining strip is the workpiece.  Both done on some form of mechanical press. Piercing (Punching) and Blanking Clearance (VIMP)  Die opening must be larger than punch and known as ‘clearance’.  Punching Punch = size of hole Die = punch size +2 clearance  Remember: In punching punch is correct size.  Blanking Die = size of product Punch = Die size -2 clearance  Remember: In blanking die size will be correct.
• 2. 7/14/2015 2 Punching Blanking Clearance Contd…. Clearance in %  If the allowance for the material is a = 0.075 given then C = 0.075 x thickness of the sheet  If clearance is 10 % given then C = 0.01 x thickness of the sheet Example Determine the die and punch sizes for blanking a circular disc of 20-mm diameter from a sheet whose thickness is 1.5 mm. Shear strength of sheet material = 294 MPa Also determine the die and punch sizes for punching a circular hole of 20-mm diameter from a sheet whose thickness is 1.5 mm. Punching Force and Blanking Force The punching force for holes which are smaller than the stock thickness may be estimated as follows: max F Lt  max 3 dt F d t    Capacity of Press for Punching and Blanking Press capacity will be = [Where C is a constant and equal to 1.1 to 1.75 depending upon the profile] m ax F C 
• 3. 7/14/2015 3 Example Estimate the blanking force to cut a blank 25 mm wide and 30 mm long from a 1.5 mm thick metal strip, if the ultimate shear strength of the material is 450 N/mm2. Also determine the work done if the percentage penetration is 25 percent of material thickness. Minimum Diameter of Piercing Piercing pressure, = Strength of punch, s d.t      2 c d 4 Energy and Power for Punching and Blanking   max Ideal Energy (E in J) maximum force x punch travel= F p t    max max (Unit:F in kNand tin mm othrwiseuseF in and tin m) Where p is percentage penetration required for rupture N   max ( ) 60 [Where N =actualnumber of stroke perminute] ( ) Where C is a constant and equal to 1.1 to 1.75 depending upon the profile ( ) 60 E N Ideal powerin press PinW Actual Energy Ein J F p t C E N Actual powerin press PinW           WhereE is actual energy and is efficiency of the press  Shear on Punch  To reduce shearing force, shear is ground on the face of the die or punch.  It distribute the cutting action over a period of time.  Shear only reduces the maximum force to be applied but total work done remains same.
• 4. 7/14/2015 4 Force required with shear on Punch Where p = penetration of punch as a fraction S = shear on the punch or die, mm    max F (tp) L t(tp) F S S Example  A hole, 100 mm diameter, is to be punched in steel plate 5.6 mm thick. The ultimate shear stress is 550 N/mm2 . With normal clearance on the tools, cutting is complete at 40 per cent penetration of the punch. Give suitable shear angle for the punch to bring the work within the capacity of a 30T press. Example A washer with a 12.7 mm internal hole and an outside diameter of 25.4 mm is to be made from 1.5 mm thick strip. The ultimate shearing strength of the material of the washer is 280 N/mm2. (a) Find the total cutting force if both punches act at the same time and no shear is applied to either punch or the die. (b) What will be the cutting force if the punches are staggered, so that only one punch acts at a time. (c) Taking 60% penetration and shear on punch of 1 mm, what will be the cutting force if both punches act together. GATE-2010 Statement Linked 1 Statement for Linked Answer Questions: In a shear cutting operation, a sheet of 5 mm thickness is cut along a length of 200 mm. The cutting blade is 400 mm long and zero-shear (S = 0) is provided on the edge. The ultimate shear strength of the sheet is 100 MPa and penetration to thickness ratio is 0.2. Neglect friction. Assuming force vs displacement curve to be rectangular, the work done (in J) is (a) 100 (b) 200 (c) 250 (d) 300 S 400
• 5. 7/14/2015 5 GATE-2010 Statement Linked 2 Statement for Linked Answer Questions: In a shear cutting operation, a sheet of 5mm thickness is cut along a length of 200 mm. The cutting blade is 400 mm long and zero-shear (S = 0) is provided on the edge. The ultimate shear strength of the sheet is 100 MPa and penetration to thickness ratio is 0.2. Neglect friction. A shear of 20 mm (S = 20 mm) is now provided on the blade. Assuming force vs displacement curve to be trapezoidal,the maximum force (in kN) exerted is (a) 5 (b) 10 (c) 20 (d) 40 S 400 Fine Blanking Fine Blanking - dies are designed that have small clearances and pressure pads that hold the material while it is sheared. The final result is blanks that have extremelyclose tolerances.  Slitting - moving rollers trace out complex paths during cutting (like a can opener).  Perforating: Multiple holes which are very small and close together are cut in flat work material.  Notching: Metal pieces are cut from the edge of a sheet, strip or blank.
• 6. 7/14/2015 6  Trimming - Cutting unwanted excess material from the periphery of a previously formed component.  Shaving - Accurate dimensions of the part are obtained by removing a thin strip of metal along the edges.  Lancing – A hole is partially cut and then one side is bent down to form a sort of tab or louver. No metal removal, no scrap.  Squeezing - Metal is caused to flow to all portions of a die cavity under the action of compressive forces.  Steel Rules - soft materials are cut with a steel strip shaped so that the edge is the pattern to be cut.  Nibbling - a single punch is moved up and down rapidly, each time cutting off a small amount of material. This allowsa simple die to cut complex slots. Dinking  Used to blank shapes from low-strength materials, such as rubber, fiber, or cloth.  The shank of a die is either struck with a hammer or mallet or the entire die is driven downward by some form of mechanical press. Elastic recovery or spring back  Total deformation = elastic deformation + plastic deformation.  At the end of a metal working operation, when the pressure is released, there is an elastic recovery and the total deformation will get reduced a little. This phenomenon is called as "spring back". Elastic recovery or spring back Contd..  More important in cold working.  It depends on the yield strength. Higher the yield strength, greater spring back.  To compensate this, the cold deformation be carried beyond the desired limit by an amount equal to the spring back.
• 7. 7/14/2015 7 Punch and Die material  Commonly used – tool steel  For high production - carbides Punching Press Bolster plate Bolster plate Contd....  When many dies are to run in the same press at different times, the wear occurring on the press bed is high. The bolster plate is incorporated to take this wear.  Relativelycheap and easy to replace.  Attached to the press bed and the die shoe is then attached to it. Punch plate  Used to locate and hold the punch in position.  This is a useful way of mounting, especially for small punches. Stripper
• 8. 7/14/2015 8 Stripper Contd....  The stripper removes the stock from the punch after a piercing or blanking operation. Ps = KLt Where Ps = stripping force, kN L = perimeter of cut, mm t = stock thickness, mm K = stripping constant, = 0.0103 for low- carbon steels thinner than 1.5 mm with the cut at the edge or near a preceding cut = 0.0145 for same materials but for other cuts = 0.0207 for low- carbon steels above 1.5-mm thickness = 0.0241 for harder materials Knockout  Knockout is a mechanism, usually connected to and operated by the press ram, for freeing a work piece from a die. Pitman  It is a connecting rod which is used to transmit motion from the main drive shaft to the press slide. Dowel pin GATE 2011 The shear strength of a sheet metal is 300 MPa. The blanking force required to produce a blank of 100 mm diameter from a 1.5 mm thick sheet is close to (a) 45 kN (b) 70 kN (c) 141 kN (d) 3500 kN
• 9. 7/14/2015 9 GATE-2002 In a blanking operation, the clearance is provided on (a) The die (b) Both the die and the punch equally (c) The punch (d) Brittle the punch nor the die GATE-2001 The cutting force in punching and blanking operationsmainlydepends on (a) The modulus of elasticity of metal (b) The shear strength of metal (c) The bulk modulusof metal (d) The yield strength of metal IAS – 2003 The 'spring back' effect in press working is (a) Elastic recovery of the sheet metal after removal of the load (b) Regaining the original shape of the sheet metal (c) Release of stored energy in the sheet metal (d) Partial recoveryof the sheet metal Drawing Drawing  Drawing is a plastic deformation process in which a flat sheet or plate is formed into a three-dimensional part with a depth more than several times the thickness of the metal.  As a punch descends into a mating die, the metal assumes the desired configuration.
• 10. 7/14/2015 10 Drawing  Hot drawing is used for thick-walled parts of simple geometries, thinning takes place.  Cold drawing uses relatively thin metal, changes the thickness very little or not at all, and produces parts in a widevariety of shapes. Blank Size 2 4 D d dh   When d > 20r       2 2 4 0.5 when15r d 20r 2 4 2 0.7 when d < 10r             D d dh r D d r d h r r d r Deep drawing  Drawing when cup height is more than half the diameter is termed deep drawing.  Easy with ductile materials.  Due to the radial flow of material, the side walls increase in thickness as the height is increased.  A cylindrical vessel with flat bottom can be deep drawn by double action deep drawing.  Deep drawing - is a combination of drawing and stretching. Stresses on Deep Drawing  In flange of blank: Bi-axial tension and compression  In wall of the cup: simple uni-axial tension Deep Drawability  The ratio of the maximum blank diameter to the diameterof the cup drawn . i.e. D/d.  There is a limiting drawing ratio (LDR), after which the punch will pierce a hole in the blank instead of drawing.  This ratio depends upon material, amount of friction present, etc.  Limiting drawing ratio (LDR) is 1.6 to 2.3
• 11. 7/14/2015 11 Limiting Drawing Ratio (LDR)  The average reduction in deep drawing 0.5 Reduction 1 100% 50% Thumb rule: First draw:Reduction 50 % Second draw:Reduction 30 % Third draw:Reduction 25% Fourth draw:Reduction 16% Fifth draw:Reduction 13% d D d D                 IES – 1997 A cup of 10 cm height and 5 cm diameter is to be made from a sheet metal of 2 mm thickness. The numberof deductions necessary will be (a) One (b) Two (c) Three (d) Four Die Design  Progressive dies  Compound dies  Combination dies Progressive dies Perform two or more operations simultaneously in a single stroke of a punch press, so that a complete component is obtained for each stroke. Compound dies All the necessary operations are carried out at a single station, in a single stroke of the ram. To do more than one set of operations, a compound die consists of the necessary sets of punches and dies. Combinationdies A combination die is same as that of a compound die with the main difference that here non-cutting operations such as bending and forming are also included as part of the operation. Progressive piercing and blanking die for making a simple washer. Back Method for making a simple washer in a compound piercing and blanking die. Part is blanked (a) and subsequently pierced (b) The blanking punch contains the die for piercing. Back
• 12. 7/14/2015 12 Lubrication  In drawing operation, proper lubrication is essential for 1. To improve die life. 2. To reduce drawing forces. 3. To reduce temperature. 4. To improve surface finish. Defects in Drawing - wrinkle  An insufficient blank holder pressure causes wrinkles to develop on the flange, which may also extend to the wall of the cup. Flange Wrinkle Wall Wrinkle Defects in Drawing - Fracture  Further, too much of a blank holder pressure and friction may cause a thinning of the walls and a fracture at the flange, bottom, and the corners (if any). Defects in Drawing -earing  While drawing a rolled stock, ears or lobes tend to occur because of the anisotropy induced by the rolling operation. Defects in Drawing – miss strike  Due to the misplacement of the stock, unsymmetrical flanges may result. This defectis known as miss strike. Defects in Drawing – Orange peel  A surface roughening (defect) encountered in forming productsfrom metal stock that has a coarse grain size.  It is due to uneven flow or to the appearance of the overly large grains usually the result of annealing at too high a temperature.
• 13. 7/14/2015 13 Stretcher strains (like Luders Lines)  Caused by plastic deformation due to inhomogeneous yielding.  These lines can criss-cross the surface of the workpiece and may be visibly objectionable.  Low carbon steel and aluminium shows more stretcher strains. Surface scratches  Die or punch not having a smooth surface, insufficient lubrication GATE-2008 In the deep drawing of cups, blanks show a tendency to wrinkle up around the periphery (flange). The most likely cause and remedy of the phenomenon are, respectively, (A) Buckling due to circumferential compression; Increase blank holder pressure (B) High blank holder pressure and high friction; Reduce blank holder pressure and apply lubricant (C) High temperature causing increase in circumferential length: Applycoolant to blank (D) Buckling due to circumferential compression; decrease blank holder pressure GATE-1999 Identify the stress - state in the FLANGE portion of a PARTIALLYDRAWN CYLINDRICAL CUP when deep - drawing withouta blank holder (a) Tensile in all three directions (b) No stress in the flange at all, because there is no blank-holder (c) Tensile stress in one direction and compressive in the one other direction (d) Compressive in two directions and tensile in the third direction GATE-2003 A shell of 100 mm diameter and 100 mm height with the corner radius of 0.4 mm is to be produced by cup drawing. The required blank diameter is (a) 118 mm (b) 161 mm (c) 224 mm (d) 312 mm
• 14. 7/14/2015 14 ISRO-2011 The initial blank diameter required to form a cylindrical cup of outside diameter 'd‘ and total height 'h' having a corner radius 'r' is obtained using the formula 2 2 2 2 ( ) 4 0.5 ( ) 2 2 ( ) 2 2 ( ) 4 0.5 o o o o a D d dh r b D d h r c D d h r d D d dh r             Spinning Spinning  Spinning is a cold-forming operation in which a rotating disk of sheet metal is shaped over a male form,or mandrel.  Localized pressure is applied through a simple round-ended wooden or metal tool or small roller, whichtraverses the entire surface of the part Spinning 1. A mandrel (or die for internal pieces) is placed on a rotating axis (like a turning center). 2. A blank or tube is held to the face of the mandrel. 3. A roller is pushed against the material near the center of rotation, and slowly moved outwards, pushing the blank against the mandrel. 4. The part conforms to the shape of the mandrel (with some springback). 5. The process is stopped, and the part is removed and trimmed. tc = tb sin
• 15. 7/14/2015 15 GATE-1992 The thickness of the blank needed to produce, by powerspinning a missilecone of thickness 1.5 mm and half cone angle 30°, is (a) 3.0 mm (b) 2.5 mm (c) 2.0 mm (d) 1.5 mm High Energy Rate Forming(HERF) HERF  High Energy Rate Forming, also known as HERF or explosive forming can be utilised to form a wide variety of metals, from aluminum to high strength alloys.  Applied a large amount of energy in a very sort time interval.  HERF makes it possible to form large work pieces and difficult-to-form metals with less-expensive equipment and tooling required.  No springback Underwater explosions. Underwater spark discharge (electro- hydraulic). Pneumatic- mechanical means Internal combustion of gaseous mixtures. Electro-magnetic (the use of rapidly formed magnetic fields). HERF Underwater Explosions Underwater explosions  A shock wave in the fluid medium (normally water ) is generated by detonating an explosive charge.  TNT and dynamite for higher energy and gun powderfor lower energy is used.  Used for parts of thick materials.  Employed in Aerospace, aircraft industries and automobile related components.
• 16. 7/14/2015 16 Electro-hydraulic Forming  An operation using electric discharge in the form of sparks to generate a shock wave in a fluid is called electrohydrulicforming.  A capacitor bank is charged through the charging circuit, subsequently, a switch is closed, resulting in a spark within the electrode gap to discharge the capacitors.  Energy level and peak pressure is lower than underwater explosionsbut easier and safer.  Used for bulging operations in small parts. Electromagnetic or Magnetic Pulse Forming  Based on the principle that the electromagnetic field of an induced current always opposes the electromagnetic field of the inducing current.  A large capacitor bank is discharged, producing a current surge through a coiled conductor.  If the coil has been placed within a conductive cylinder, around a cylinder, or adjacent the flat sheet of metal, the discharge induces a secondary current in the workpiece, causing it to be repelled from the coil and conformed to a die or mating workpiece. Electromagnetic or Magnetic Pulse Forming  The process is very rapid and is used primarily to expand or contract tubing, or to permanently assemble componentparts.  This process is most effective for relatively thin materials (0.25 to 1.25 mm thick). IES 2011 High energy rate forming process used for forming components from thin metal sheets or deform thin tubes is: (a) Petro-forming (b) Magnetic pulse forming (c) Explosive forming (d) electro-hydraulicforming
• 17. 7/14/2015 17 JWM 2010 Assertion (A) : In magnetic pulse-forming method, magnetic field produced by eddy currents is used to create force between coil and workpiece. Reason (R) : It is necessary for the workpiece material to have magnetic properties. (a) Both A and R are individually true and R is the correctexplanation of A (b) Both A and R are individually true but R is NOT the correctexplanation of A (c) A is true but R is false (d) A is false but R is true IES 2010 Assertion (A) : In the high energy rate forming method, the explosive forming has proved to be an excellent method of utilizing energy at high rate and utilizes both the high explosives and low explosives. Reason (R): The gas pressure and rate of detonation can be controlled for both types of explosives. (a) Both A and R are individually true and R is the correct explanation of A (b) Both A and R are individually true but R is NOT the correct explanation of A (c) A is true but R is false (d) A is false but R is true IES – 2007 Which one of the following metal forming processes is not a high energy rate forming process? (a) Electro-mechanical forming (b) Roll-forming (c) Explosive forming (d) Electro-hydraulicforming IES – 2009 Which one of the following is a high energy rate formingprocess? (a) Roll forming (b) Electro-hydraulicforming (c) Rotary forging (d) Forwardextrusion IES – 2005 Magneticforming is an example of: (a) Cold forming (b) Hot forming (c) High energy rate forming (d) Roll forming Stretch Forming  Produce large sheet metal parts in low or limited quantities.  A sheet of metal is gripped by two or more sets of jaws that stretch it and wrap it around a single form block.  Because most of the deformation is induced by the tensile stretching, the forces on the form block are far less than those normally encountered in bending or forming.  There is very little springback, and the workpiece conformsvery closely to the shape of the tool.  Because the forces are so low, the form blocks can often be made of wood, low-melting-point metal, or even plastic.
• 18. 7/14/2015 18 Stretch Forming Contd......  Popular in the aircraft industry and is frequently used to formaluminum and stainless steel  Low-carbon steel can be stretch formed to produce large panels for the automotive and truck industry. Stretch Forming Contd...... Stretch Forming Contd...... GATE-2000 A 1.5 mm thick sheet is subject to unequal biaxial stretching and the true strains in the directions of stretching are 0.05 and 0.09. The final thickness of thesheet in mm is (a) 1.414 (b) 1.304 (c) 1.362 (d) 289 Ironing  The process of thinning the walls of a drawn cylinder by passing it between a punch and die whose separation is less than the original wall thickness.  The walls are thinned and lengthened, while the thickness of the base remains unchanged.  Examples of ironed products include brass cartridge cases and the thin-walled beverage can.
• 19. 7/14/2015 19 Ironing Contd.... Embossing  It is a very shallow drawing operation where the depth of the draw is limited to one to three times the thickness of the metal, and the material thickness remains largely unchanged. Coining  Coining is essentially a cold-forging operation except for the fact that the flow of the metal occurs only at the top layers and not the entire volume.  Coining is used for making coins, medals and similar articles. Bending  After basic shearing operation, we can bend a part to give it some shape.  Bending parts depends upon material properties at the location of the bend.  At bend, bi-axial compression and bi-axial tension is there. Bending Bend allowance, Lb = α(R+kt) where R = bend radius k = constant (stretch factor) t = thickness of material α = bend angle (in radian) 2 0.5 2 0.33 For R t k For R t k     Bending  The strain on the outermost fibers of the bend is 1 2 1 r t   
• 20. 7/14/2015 20 Bending Force Condition V-Bending U-Bending Edge-Bending W < 16t 1.33 2.67 0.67 W > = 16t 1.20 2.40 0.6 2 ut Where l=Bend length =width of thestock,mm σ = Ultimate tensilestrength,MPa (N/mm ) t = blank thickness, mm w =width of die-opening,mm K =die-opening factor ,(can be usedfollowin table) 2 ut Kl t F w   For U or channel bending force required is double than V – bending For edge bending it will be about one-half that for V - bending GATE-2005 A 2 mm thick metal sheet is to be bent at an angle of one radian with a bend radius of 100 mm. If the stretch factor is 0.5, the bend allowance is (a) 99 mm (b) 100 mm (c) 101 mm (d) 102 mm 2mm 1 radian GATE -2012 Same Q in GATE-2012 (PI) Match the following metal forming processes with their associated stresses in the workpiece. (a) 1-S, 2-P, 3-Q, 4-R (b) 1-S, 2-P, 3-R, 4-Q (c) 1-P, 2-Q, 3-S, 4-R (d) 1-P, 2-R, 3-Q, 4-S Metal forming process Typeof stress 1. Coining P. Tensile 2. Wire Drawing Q. Shear 3. Blanking R. Tensile and compressive 4. Deep Drawing S. Compressive